- Email: [email protected]

Contents lists available at ScienceDirect

European Journal of Mechanics A/Solids journal homepage: www.elsevier.com/locate/ejmsol

A modiﬁed Gurson model to account for the inﬂuence of the Lode parameter at high triaxialities ndez-Sa ez G. Vadillo*, J. Reboul, J. Ferna Department of Continuum Mechanics and Structural Analysis, University Carlos III of Madrid, Avda. de la Universidad, 30, 28911 Legan es, Madrid, Spain

a r t i c l e i n f o

a b s t r a c t

Article history: Received 18 March 2015 Accepted 22 September 2015 Available online 22 October 2015

The inﬂuence of the Lode parameter on ductile failure has been pointed out by different authors even at high triaxiality stress states. However, one of the most widely used model for ductile damage, like the GursoneTvergaard (GT) model, systematically disregard the role played by the third stress invariant. In this paper, an improvement of the classical GursoneTvergaard model is proposed. The new relation takes into account the effect of triaxiality and Lode parameter through the q1 and q2 GT parameters. The convexity of the proposed yield surface has been examined and ensured. The integration of the new constitutive equations as well as the consistent tangent modulus have been formulated and implemented in a Finite Element code. A computational 3D cell has been used to prescribe both macroscopic triaxiality and Lode parameter during loading. Numerical simulations are presented for Weldox 960 steel with different initial porosities and for different prescribed macroscopic triaxialities and Lode parameters using a computational 3D cell methodology. The results are compared with those obtained with a J2 voided cell. These comparisons show that the improved model captures adequately the Lode effect on the stress-strain curves and on the void growth. © 2015 Elsevier Masson SAS. All rights reserved.

Keywords: Gurson model Lode parameter Cell model analysis

1. Introduction The ductile fracture phenomenon in metals and alloys usually follows a failure mechanism involving nucleation, growth and coalescence of voids. Pioneering micromechanical studies of this phenomenon were carried out by McClintock (1968), Rice and Tracey (1969), considering the growth of isolated cylindrical or spherical voids driven by plastic deformation of the surrounding rigid perfectly plastic matrix material. To analyze the ductile failure of porous materials, the GursoneTvergaard (GT) damage model (Gurson, 1977; Tvergaard, 1981, 1982) is the most widely used approach. Tvergaard (1981, 1982) modiﬁed the Gurson model by introducing the q1 and q2 parameters to more accurately describe the void growth kinetics observed in unit cell computations. Faleskog et al. (1998) and Gao et al. (1998) have shown that these values are not constant but depend on both strength and strainhardening properties. More recently, Kim et al. (2004) and Vadillo ndez-S and Ferna aez (2009) have pointed out that the qi parameters also depend on the triaxiality of the stress ﬁeld, as well as on the

* Corresponding author. Tel.: þ34 916248460; fax: þ34 916249430. E-mail address: [email protected] (G. Vadillo). http://dx.doi.org/10.1016/j.euromechsol.2015.09.010 0997-7538/© 2015 Elsevier Masson SAS. All rights reserved.

initial porosity, and highlighted the importance of a proper choice of q1 and q2 for the correct modelling of the void growth process. Various extensions of the Gurson model have been developed and provided elsewhere in order to better represent the response of ra jeu et al., 2000; Pardoen ductile metals (Gologanu et al., 1997; Ga and Hutchinson, 2000; Zhang et al., 2000; Benzerga, 2002; Flandi and Leblond, 2005; Monchiet et al., 2008). These modiﬁcations make all the assumption of axisymmetric cavities remaining spheroidal during plastic deformation. For a review on constitutive models developed to simulate ductile failure see Besson (2010), Pineau and Pardoen (2007). In the last years, several researchers (Zhang et al., 2001; Kim et al., 2003, 2004; Bao and Wierzbicki, 2004; Wen et al., 2005; Gao and Kim, 2006; Kim et al., 2007; Xue, 2007; Barsoum and Faleskog, 2007; Xue, 2008; Bai and Wierzbicki, 2008; Brünig et al., 2008; Gao et al., 2009, 2011; Barsoum and Faleskog, 2011; Barsoum et al., 2011; Jackiewicz, 2011; Danas and Ponte~ eda, 2012; Benallal et al., 2014) outlined that the stress Castan triaxiality measure by itself is insufﬁcient to characterize plastic yielding, and highlighted the role of the third invariant of the deviatoric stress tensor, on void growth rates and other aspects of void behaviour which play an important role in strain softening and localization.

32

G. Vadillo et al. / European Journal of Mechanics A/Solids 56 (2016) 31e44

At high triaxialities, where the controlling damage mechanism is the void growth, the inﬂuence of Lode parameter can be also important (Barsoum et al., 2011). This effect cannot be properly accounted for with the classical GT model. At low triaxialities, the source of the instability cannot be identiﬁed with a void growth mechanism (Yamamoto, 1978). The GT model was recently modiﬁed to introduce a Lode dependent softening term for low triaxialities (Nahshon and Hutchinson, 2008). By construction, this modiﬁcation is inconsistent with mass conservation (Danas and ~ eda, 2012). Ponte-Castan In the present paper, an improvement of the GursoneTvergaard model that accounts for the inﬂuence of the Lode parameter at high triaxiality stress states is presented. The modiﬁcation consists on incorporating the Lode parameter effect into the GT yield surface through q1 and q2, which depend not only of the stress triaxiality T, but also on the third invariant of the deviatoric stress tensor J3. This new term is calibrated to ensure the convexity of the yield surface. The integration of the new constitutive equations has been implemented using a full implicit Eulerbackward scheme combined with the return mapping algorithm. Additionally, the consistent tangent modulus has been formulated. For validation purposes, a 3D extension of the computational cell model employed by Xia and Shih (1995a,b, 1996) has been developed extending the prescription to both macroscopic triaxiality and Lode parameter. Numerical simulations using the Finite Element code ABAQUS/Standard (Simulia, 2014) are presented for Weldox 960 steel considering different initial porosities and various prescribed macroscopic triaxialities and Lode values. The obtained results using the new continuum damage model are compared with those found with a J2 voided cell for both the void growth and the stress-strain response of the material.

2. Unit-3D cell model with prescribed triaxiality and Lode parameter

u1 ¼ 0 at x1 ¼ 0; u2 ¼ 0 at x2 ¼ 0; u3 ¼ 0 at x3 ¼ 0;

u1 ¼ U1 at x1 ¼ D1 ; u2 ¼ U2 at x2 ¼ D2 ; u3 ¼ U3 at x3 ¼ D3 ;

(1)

The macroscopic logarithmic principal strains have the form:

E1 ¼ ln

D1 ; D01

E2 ¼ ln

D2 ; D02

E3 ¼ ln

D3 D03

(2)

and the effective strain:

pﬃﬃﬃ 1=2 2 ðE1 E2 Þ2 þ ðE1 E3 Þ2 þ ðE2 E3 Þ2 Ee ¼ 3

(3)

with the rates of macroscopic logarithmic principal strains given by:

D_ E_ 1 ¼ 1 ; D1

D_ E_ 2 ¼ 2 ; D2

D_ E_ 3 ¼ 3 D3

(4)

where D1 ¼ D01 þ U1, D2 ¼ D02 þ U2 and D3 ¼ D03 þ U3 are the current lengths of the representative deformed cell. The macroscopic principal stresses, S1, S2 and S3 are deﬁned as:

Si ¼

1 Dj Dk

ZDj ZDk ½sii xi ¼Di dxj dxk 0

with i; j; k ¼ 1; 2; 3

0

sii being the Cauchy stress components, and Se and Sh, the effective and hydrostatic macroscopic stresses: 1=2 1 Se ¼ pﬃﬃﬃ ðS1 S2 Þ2 þ ðS1 S3 Þ2 þ ðS2 S3 Þ2 ; 2 S þ S2 þ S3 Sh ¼ 1 3

(5)

The stress triaxiality T and the Lode parameter L can be written as:

2.1. The unit-cell model Under the assumption of a periodic microstructure, a porous material can be approximated by representative volume elements (RVE), each containing a void. The axisymmetric cell model is a very convenient way to simplify the problem, because it requires only two-dimensional calculations, so is the most frequently way to analyse the material behaviour. Those authors who only deal with axisymmetric conditions ignore the inﬂuence of other possible Lode parameter values in the response of the material. To analyse the inﬂuence of the Lode parameter, a cubic 3D cell in which a spherical void is contained should be considered (Zhang et al., 2001; Kim et al., 2007). In this paper, a unit cell with initial lengths 2D01, 2D02 and 2D03 and a spherical void located at its center of radius r0 is chosen. The RVE will be modelled by two approaches, one governed by the classical J2 plasticity with a cell containing a discrete spherical void and another considering a homogeneous continuum damage model cell with the same initial void volume fraction as the voided one ðf0 ¼ pr03 =ð6D01 D02 D03 ÞÞ. Both cells are subjected to the same macroscopic loading history, obtained prescribing the displacements on the outer surfaces of each unitary cell. In both cases all boundaries are shear traction free, and the void surface in J2 unit cell is also traction free, as shown in Fig. 1. Due to symmetry of the problem, only the eighth part of the region needs to be modelled. Assuming that the outer surfaces are always parallel to the 1, 2 and 3 directions respectively, the boundary conditions at the cell during the deformation process are:

T¼

Sh ; Se

L¼

2S2 S1 S3 S1 S3

(6)

Deﬁning the following ratios between S1, S2 and S3:

R¼

S2 ; S1

Q¼

S3 S1

(7)

the stress triaxiality, T, and the Lode parameter, L, are given by:

pﬃﬃﬃ 2ðR þ Q þ 1Þ T ¼ qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ; 2 3 ð1 RÞ þ ð1 Q Þ2 þ ðR Q Þ2

L¼

2R Q 1 1Q

(8)

2.2. Boundary conditions for prescribing triaxiality and Lode parameters In order to study the effect of stress triaxiality T and Lode parameter L in the mechanical behaviour of the representative volume element, boundary conditions should be implemented to prescribe the ratios of the principal stresses R ¼ S2/S1 and Q ¼ S3/ S1 during the whole loading history of the RVE. Faleskog et al. (1998) developed a method to prescribe displacement rates in a 3D unitary cell under plane strain condition which results in a constant macroscopic triaxiality. In this work, this strategy is extended to prescribe both triaxiality and Lode

G. Vadillo et al. / European Journal of Mechanics A/Solids 56 (2016) 31e44

33

Fig. 1. Geometry and displacements imposed as boundary conditions on the unitary J2 voided cell and on the continuum damage model cell.

parameter during the entire deformation history of the 3D unitary cell. In the voided J2 cell, the macroscopic stresses Si are calculated as the average stress on the cell boundaries. In the continuum damage model cell, Si are the macroscopic stress in the prevailing homogeneous stress ﬁeld. Since the macroscopic true stresses (S1, S2, S3) and the macroscopic strain rates (E_ 1 , E_ 2 , E_ 3 ) are equal to the volume average values in a cell (Hill, 1967), the total rate of deformation _ in both continuum damage model cell (CC) and J2 voided work W cell (VC), can be written as:

_ _ _ _ _ W CC ¼ W VC ¼ VS1 E1 þ VS2 E2 þ VS3 E3

(9)

V being the present volume of each cell. Deﬁning P1 ¼ VS1, P2 ¼ VS2 and P3 ¼ VS3 as generalized forces and work rate conjugate quantities to E_ 1 , E_ 2 and E_ 3 , respectively, the above expression becomes:

_ _ _ _ _ W CC ¼ W VC ¼ P1 E1 þ P2 E2 þ P3 E3

(10)

1 R Q A11 ¼ qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ; A12 ¼ qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ; A13 ¼ qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2 2 2 2 1þR þQ 1þR þQ 1 þ R2 þ Q 2 R 1 A21 ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ; A22 ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ; A23 ¼ 0: 2 1þR 1 þ R2 Q RQ A31 ¼ qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ﬃ; A32 ¼ qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ﬃ 2 2 2 2 1þR 1þR þQ 1 þ R 1 þ R2 þ Q 2 1 þ R2 A33 ¼ qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ﬃ 1 þ R2 1 þ R2 þ Q 2 (12) _ _ The total rate of deformation work (W CC and W VC ) can be expressed as:

_ _ _ _ _ W CC ¼ W VC ¼ PðIÞ EðIÞ þ PðIIÞ EðIIÞ þ PðIIIÞ E ðIIIÞ

(13)

If in the transformed coordinate system, the imposed incremental boundary conditions are stress uniaxial:

in which the generalized forces P1, P2 and P3 should satisfy, to prescribe the ratios of principal stresses R ¼ S2/S1 and Q ¼ S3/S1, the relations P2/P1 ¼ R; P3/P1 ¼ Q. Consider the transformation:

E_ ðIÞ ¼ E_ I ;

0

The total rate of deformation work has in this system the form _ _ _ W CC ¼ W VC ¼ PðIÞ EI , that follows, in the original one and considering the relations given in Eq. (11), the three relations:

1 0 1 E_ ðIÞ E_ 1 B _ C @ ¼ N E @ ðIIÞ A E_ 2 A; _ E_ 3 E ðIIIÞ

0

1

0

1

PðIÞ P1 @ PðIIÞ A ¼ [email protected] P2 A PðIIIÞ P3

(11)

N being an orthonormal (N1 ¼ NT) unsymmetric matrix of the form:

0

A11 N ¼ @ A21 A31

A12 A22 A32

with elements:

1 A13 A23 A; A33

ð1Þ ð2Þ ð3Þ

PðIIÞ ¼ 0;

PðIIIÞ ¼ 0

E_ ðIÞ ¼ E_ I /A11 E_ 1 þ A12 E_ 2 þ A13 E_ 3 ¼ E_ I PðIIÞ ¼ 0/A21 P1 þ A22 P2 þ A23 P3 ¼ 0 PðIIIÞ ¼ 0/A31 P1 þ A32 P2 þ A33 P3 ¼ 0

(14)

(15)

or in a similar manner:

ð1Þ ð2Þ ð3Þ

E_ 1 þ RE_ 2 þ Q E_ 3 ¼ E_ I RS1 ¼ S2 Q S1 ¼ S3

qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 þ R2 þ Q 2

(16)

34

G. Vadillo et al. / European Journal of Mechanics A/Solids 56 (2016) 31e44

For given values of R, Q and E_ I , imposing the three boundary conditions in the transformed system of each cell (E_ ðIÞ ¼ E_ I , P(II) ¼ 0, P(III) ¼ 0), lead to prescribe, in both continuum damage model cell (CC) and J2 voided cell (VC) of the original system, the relations:

ð1Þ

E_ 1 þ RE_ 2 þ Q E_ 3

ð2Þ ð3Þ

ðS2 =S1 ÞCC ¼ ðS2 =S1 ÞVC ¼ R ðS3 =S1 ÞCC ¼ ðS3 =S1 ÞVC ¼ Q

CC

¼ E_ 1 þ RE_ 2 þ Q E_ 3

VC

(17)

with R and Q, from Eq. (8) and for S3 < S1, as functions of T and L. The boundary conditions are implemented in ABAQUS/Standard (Simulia, 2014) via a MPC subroutine. This method overcomes difﬁculties associated with cell softening due to void growth. 3. Numerical cell results for the voided J2 and for the classical GursoneTvergaard model Many authors (Zhang et al., 2001; Kim et al., 2007; Gao et al., 2005; Xue, 2008) show that a voided cell subjected to the same stress triaxiality ratio, would tends to react differently when Lode parameter is different. In this section, we will discuss the macroscopic stress-strain evolution and the growth of the porosity (until coalescence) of a voided J2 cell subjected to prescribed triaxiality and Lode parameter values during the deformation history. For this purpose, the range of high stress triaxialities (1 T 2) and L values within the range (1 L 1) are analyzed. The chosen material for the analysis is Weldox 960, material which presents a Lode parameter dependence behaviour as was experimentally proved by Barsoum et al. (2011). The following true stress-strain relation can approximate the high strength steel behaviour:

8 Eε > <

ε ε0 s¼ ε N > : s0 ε > ε0 ε0

(18)

where s0 represents the initial yield stress, N the strain hardening exponent and ε0 ¼ s0/E, E being the Young Modulus. All material properties are listed in Table 1. It should be noted that at high triaxiality level, the prediction of ductile fracture depends on void growth, which is clearly different from the mechanism leading to failure at the low positive or negative hydrostatic stress ﬁelds (T values not considered in this work). 3.1. J2 voided cell results The RVE voided cell considered in this study has the initial length ratios D01/D02 ¼ D01/D03 ¼ 1, and two initial void volume fractions f0 ¼ 0.005 and f0 ¼ 0.01 are analyzed. The ﬁnite element mesh used in the calculations for f0 ¼ 0.005 is shown in Fig. 2, and consists of 8680 eight-node linear brick hexaedrical elements with reduced integration and hourglass control. This mesh includes 22 elements in the intersection of each outer surfaces with the void surface, and 20 elements along each longitudinal direction. The numerical analyses of the Weldox 960 material that obeys the

Table 1 Material properties of Weldox 960. E(GPa)

n

s0 (MPa)

N

ε0

208

0.3

956

0.059

0.0046

Fig. 2. Example of the ﬁnite element mesh of a cell with initial void volume fraction f0 ¼ 0.005.

theory of J2 plasticity are carried out using the Finite Element code ABAQUS/Standard (Simulia, 2014) within an updated Lagrangian formulation. The nonlinear boundary conditions are prescribed following the method presented in previous section. Fig. 3(a) illustrates the evolution of the macroscopic effective stress versus effective strain curve for T ¼ 1, initial void volume fraction f0 ¼ 0.005 and Lode parameters L ¼ 1, 0.5, 0.2, 0, 0.2, 0.5, 1. The competition between matrix material strain hardening and porosity induced softening is showed. As macroscopic effective deformation increases, a maximum Se/s0 value is reached, and the macroscopic effective stress decreases as strain-hardening of matrix material is insufﬁcient to be balanced for a reduction in the cell ligament area caused by void expansion. When the Lode parameter has the minimum value (L ¼ 1), the stress carrying capacity of the cell is reduced at lower Ee, whereas when L ¼ 1, the stress carrying capacity of the cell is lost much later (Zhang et al., 2001). The larger the L, the slower the lost of carrying capacity. The differences in the lost carrying capacity strongly depend of the evolution of the porosity f. As shown in Fig. 3(b), the larger the value of L tested, the smaller the increment of void volume fraction reached. Similar behaviour can be found for other high triaxialities tested. The rapid drop of stress carrying capacity and the fast increase of porosity f is marked with a circle in Fig. 3(a) and (b) deﬁning the onset of void coalescence. Following the procedure developed by Koplik and Needleman (1988) and Kim et al. (2004) for axisymmetric deformation mode, the evolution of ligament length ratios (Di Di0)/Di0 in direction i ¼ 1, 2 and 3 is represented as a function of Ee in Fig. 4 for f0 ¼ 0.005, T ¼ 1 and L ¼ 1, 0. The value of deformation where the evolution of ligament stretching stops in one (or two) directions and a rapid deformation in one (or two) directions take place, capture ﬂow localization and the beginning of coalescence. Not only void growth and critical strain for void instability are inﬂuenced by Lode parameter, also the expansion of the void can adopt different shapes for different L values under the same triaxiality level. It is well known that the inﬂuence of L on the deformation is more important at small values of T than at higher ones (Zhang et al., 2001). For high triaxialities, the shape of the voids remain nearly spherical for every L value analyzed.

G. Vadillo et al. / European Journal of Mechanics A/Solids 56 (2016) 31e44

35

Fig. 3. Evolution of macroscopic effective stress (a) and void volume fraction (b) versus macroscopic effective strain with different prescribed Lode parameters for f0 ¼ 0.005 and T ¼ 1.

Fig. 4. Variation of the deformed cell length ratio in directions i ¼ 1, 2 and 3 vs. Ee for f0 ¼ 0.005, T ¼ 1 and L ¼ 1, 0 revealing in each case a shift (circle) which corresponds to ﬂow localization.

3.2. Classical GursoneTvergaard cell results The yield function of the GursoneTvergaard (GT) model has the form:

FðSe ; Sh ; s; f Þ ¼

S2e 3q2 Sh 2 2 1 þ q þ 2q fcosh f 1 1 2s s2

(19)

f being the current void volume fraction, s the current ﬂow stress of the matrix material, and Se and Sh the effective and hydrostatic macroscopic Cauchy stresses:

Se ¼

rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 3 0 S : S0 2

;

Sh ¼

1 S:1 3

;

S0 ¼ S Sh 1

(20)

The parameters q1 and q2 were introduced by Tvergaard (1981, 1982) to improve model predictions. The GT model does not capture the effect of the coalescence phase. The material behaviour in this phase prior to separation is not considered in this work. The (q1, q2) GursoneTvergaard parameters strongly depend of material properties (Gao et al., 1998; Faleskog et al., 1998), and also are function of the initial void volume fraction f0 and of the stress ndez-Sa ez, triaxiality ratio T (Kim et al., 2004; Vadillo and Ferna 2009). The proper selection of these two parameters are critical for the accurate representation of the ductile fracture of materials. The (q1, q2) values should be calibrated to match the stress-strain response and the void growth rate of the GT cell and that predicted by the J2 voided cell analysis. To minimize the differences between the two models, and for calibration purposes, two error functions are introduced, namely:

I F F II Rf ¼ FI

RW

I W W II ¼ WI

(21)

where F denotes the area under the curve of porosity f versus Ee, Z Ec ðF ¼ fdEe Þ, and W the area under the curve of the effective 0 Z Ec ðSe =s0 ÞdEe Þ. Ec is the effective strain stress versus Ee, ðW ¼ 0

when coalescence is reached. Superscripts I and II refer to the voided cell and the GT model. F I F II and W I W II are respectively the areas between both curves in f vs. Ee and Se vs. Ee schemes (blue zone in Fig. 5(a) and (b)). Following Aravas (1987), a consistent integration procedure is used to integrate the GT model equations for Weldox 960. With the use of the backward Euler integration scheme, a numerical algorithm implicit in all variables is developed. The proposed algorithm as well as the corresponding tangent modulus is implemented in the Finite Element commercial code ABAQUS/Standard (Simulia, 2014) through a UMAT user subroutine. It was already mentioned for the voided cell model that, in the case that both triaxiality and initial void volume fraction remain constant, the macroscopic stress-strain curves, the void growth rate and the coalescence strain differs markedly for every Lode parameter analyzed. In this work, and to calibrate GT parameters for ﬁxed and constant T and f0, the Lode parameter is chosen to be the one which gives earlier coalescence (L ¼ 1) for all the cases tested.

36

G. Vadillo et al. / European Journal of Mechanics A/Solids 56 (2016) 31e44

Fig. 5. Fitting squemes for Se vs. Ee and f vs. Ee, (a) and (b), and example of calibration procedure for q1 and q2 parameters for f0 ¼ 0.005, T ¼ 1 and L ¼ 1 (c).

For a given initial porosity, T and L, different pairs of (q1, q2) values give the same prediction for the error functions: Rf ¼ TOL and RW ¼ TOL, with the chosen TOL ¼ 0.01. Fig. 5(c) shows, for f0 ¼ 0.005, T ¼ 1 and L ¼ 1, the relations q1eq2 that minimize both Rf and RW. The optimal choice for q1, q2 are obtained by the intersection of both curves. The q1 and q2 values are in this case q1 ¼ 0.855 and q2 ¼ 1.175. A summary of the optimal GT parameters for two initial porosities f0 ¼ 0.005, f0 ¼ 0.01 and two different triaxialities 1 and 2 is given in Table 2. As mentioned, in all cases the chosen Lode parameter used for calibration purposes was L ¼ 1. The coalescence strain Ec obtained from the voided cell and necessary for the calibration method is also given. For simplicity, qi(T) can be assumed to vary following a linear ndez-Sa ez, 2009): function of the form (Vadillo and Ferna

qi ðTÞ ¼ Ai T þ Bi

(22)

Table 2 Optimal q1, q2 and Ec for T ¼ 1, 2, and interpolation coefﬁcients of qi(T) for f0 ¼ 0.005 and 0.01. f0 ¼ 0.005

with the interpolation coefﬁcients Ai and Bi given in Table 2. Is a matter for discussion how to ensure yield surface convexity. Many authors test the convexity of the yield surface in a simple way, namely by plotting its two-dimensional projection at different loading stages (Pietryga et al., 2012). By taking advantage of this way, in the present work, convexity of the yield function is conﬁrmed within the range of triaxialities 1 T 2 and L ¼ 1 for porosities f0 f 0.08 for the initial void volume fractions f0 ¼ 0.005 and 0.01. Fig. 6 compares the evolution of macroscopic stress-strain and the predicted void-volume fraction growth till coalescence using GT model with calibrated qi parameters (Table 2) using the results of the J2 voided cell model. The cases analyzed corresponds to f0 ¼ 0.005, T ¼ 1, 2 and L ¼ 1, 0 and 1. It can be seen how the classical GT model, Lode independent, predicts the same behavior for different stress states when the triaxiality ratio is the same, meanwhile voided J2 cell response differs when Lode parameter changes. It is observed, for every triaxiality studied, how the difference between the two models increase when the value of the Lode parameter increases.

4. Modiﬁed GursoneTvergaard model with Lode parameter dependence

f0 ¼ 0.01

T

1

2

1

2

q1 q2 Ec

0.855 1.175 0.580

1.455 0.992 0.160

1.011 1.104 0.480

1.583 0.957 0.130

f0

A1

B1

A2

B2

0.005 0.01

0.600 0.572

0.255 0.439

0.183 0.147

1.358 1.251

q1(T)

q2(T)

4.1. Constitutive equations One of the major limitations of the GT model is that, although it is extensively used, it can only handle the growth of spherical voids remaining spherical, which is only approximately true for L ¼ 1 and at triaxialities around 1.5. However, at high triaxialities, it is possible to calibrate q1 and q2 parameters in GT model to reproduce the behavior of the material in these stress situations. These calibrated qi values are not constants, but dependent on the material,

G. Vadillo et al. / European Journal of Mechanics A/Solids 56 (2016) 31e44

37

Fig. 6. Comparison of Se vs. Ee curve and f vs. Ee curve for a voided cell and a continuum GT cell with different calibrated qi parameters. Here, f0 ¼ 0.005, T ¼ 1, 2 and L ¼ 1, 0, 1.

the stress triaxiality ratio and the initial void volume fraction ndez-Sa ez, 2009). considered (Kim et al., 2004; Vadillo and Ferna J2 cell model analysis conducted in previous sections show that the macroscopic stress-strain response and the void growth behaviour not only depend on the ﬁrst and the second stress invariants, but also on the Lode parameter (third stress invariant). However, the original GT model predicts the same void growth rate and macroscopic stress-strain response for different Lode parameter values as long as the stress triaxiality ratio T remains the same. At low triaxialities Nahshon and Hutchinson, (2008) have proposed a modiﬁcation of the Gurson model to capture softening in shear. The modiﬁcation takes into account the third invariant of the stress deviator. At high triaxialities, and in order to account for the inﬂuence of T and L on the response of the material, the main innovative feature of this work is to propose a modiﬁcation of the yield function of the classical GT model (Eq. (19)) introducing new dependences in q1 and q2 GursoneTvergaard parameters as functions of triaxiality and U. The proposed yield function has the form:

3q2mod Sh Fmod ðSe ; Sh ; T; U; s; f Þ ¼ þ 2q1mod fcosh 2s 2 2 1 þ ðq1mod Þ f S2e s2

(23)

with q1mod, q2mod, for the sake of simplicity, deﬁned as linear functions of T and U as:

q1mod ðT; UÞ ¼ q1 ðTÞ,ð1 þ kU ,UÞ;

(24)

q2mod ðT; UÞ ¼ q2 ðTÞ,ð1 þ kU ,UÞ

(25)

The functions q1(T) and q2(T) in q1mod and q2mod follows (Eq. (22)) with Ai and Bi interpolated coefﬁcients based of ﬁtted discrete qi values obtained from the axisymmetric stress state ﬁeld (U ¼ 0). U is a stress measure, function of the effective stress Se and J3 as:

U¼

27J3 2S3e

1;

J3 ¼ detðS0 Þ

lying in the range 2 U 0, with U ¼ 0 for L ¼ 1, and U ¼ 2 for L ¼ 1. kU is a proposed adjustment parameter. This modiﬁcation is

purely phenomenological, but formulated to retrieve the original GT formulation for L ¼ 1 and T ¼ constant. For hypoelastic-plastic materials, the relation between the _ and the plastic part of the rate of macroscopic stress rate, S, p macroscopic deformation E_ is given by:

_ ¼ C : E_ E_ p S

(26)

E_ being the macroscopic rate of deformation tensor and C ¼ 2GI0 þ K151 the fourth-order tensor of isotropic elastic moduli. G and K are the Shear and Bulk modulus respectively, I0 the unit deviatoric fourth order tensor and 1 the unit second order tensor. p The plastic part of the rate of macroscopic deformation E_ is derived from the associated ﬂow rule:

vFmod p E_ ¼ l_ vS

(27)

l_ being the plastic ﬂow proportionality factor, and Fmod the GT yield condition modiﬁed in this work to take into account the inﬂuence of the Lode parameter on the ductile behaviour of elasto-plastic porous materials. The plastic part of the macroscopic strain rate and the effective plastic strain rate are related by enforcing equality between the rates of macroscopic and matrix plastic work: p S : E_ ¼ ð1 f Þs ε_ p

(28)

Here, the ﬂow stress of the matrix material s and the effective p microscopic plastic strain rate ε_ are related by the law s ¼ sðεp Þ Rt p with εp ¼ 0 ε_ ðtÞdt, The evolution of porosity can be written as: p f_ ¼ ð1 f ÞE_ : 1

(29)

One should note that the evolution law for the void volume fraction is affected by the deﬁnition of the yield surface, having a dependence with Lode parameter as far as the yield function does. The above formulation must be complemented with the KuhneTucker conditions:

38

G. Vadillo et al. / European Journal of Mechanics A/Solids 56 (2016) 31e44

vT vSh vT vSe

5. Numerical implementation

vFmod vFmod Dεp ¼ Dl þ vSh vT vFmod vFmod Dεq ¼ Dl þ vSe vT vFmod DεU ¼ Dl vU

5.1. Integration procedure

that leads, after combining the above relations to eliminate Dl:

_ mod ¼ 0 l_ 0; Fmod 0; lF

(30)

_ mod ¼ 0. and the consistency condition during plastic loading: F

In the context of the Finite-Element method, the integration process is local in space and occurs at each quadrature points of the ﬁnite elements. The incremental integration of the constitutive equations is a strain-driven process in which the total strain tensor _ is given at a time (n) and increment at each quadrature point, E, both the stress tensor and the state variables should be updated at time (n þ 1). To integrate the set of non-linear constitutive Eqs. (26)e(30), two different tasks must be accomplished. The ﬁrst one consists in update stress and state variables driven by the strain increment. The second is related to deﬁne a consistent tangent modulus to preserve the quadratic convergence of the iterative solution based on Newton's method. All variables are evaluated in (n þ 1), omitting the subscript for simplicity. For the ﬁrst assignment, the classical return mapping algorithm is used (Simo and Taylor, 1985). Following a fully Backward-Euler scheme, the constitutive relations can be written in the following incremental form: From the time derivative of the generalized Hooke's law (Eq. (26)):

S ¼ Strial C : DEp

with

(35)

Strial ¼ SðnÞ þ C : DE

vFmod vFmod vT vFmod vFmod vT þ þ Dεq ¼ 0; vSe vT vSe vSh vT vSh vF vFmod vFmod vT ¼0 Dεq mod DεU þ vU vSe vT vSe Dεp

(36)

Taking into account the identity:

S0 : cofðS0 Þ ¼ 3J3

(37)

vU is equal to zero it is possible to prove that the product S0 : vS allowing the constitutive relations to be written as:

Macroscopic and matrix plastic work equivalence: Sh Dεp þ Se Dεq ¼ ð1 f ÞsDεp Void volume fraction evolution equation: Df ¼ (1 f)Dεp Kuhn-Tucker condition for plastic loading: DFmod ¼ 0 Substituting Eq. (34) into the deviatoric part of Eq. (31), the updated deviatoric stress has the form:

S0 ¼ S0trial 3GDεq

S0 Se

! 81 J3 3 S0 27 1 2 0 S 2GDεU $ þ cof ð S Þ þ 1 2 S4e 2 Se 2S3e 9 e

(31) with

From the ﬂow rule (Eq. (27)):

S0trial ¼ S0ðnÞ þ 2GI0 : DE vF 1 vFmod vFmod vT DE ¼ Dl mod ¼ Dl þ 1 3 vS vSh vT vSh

XS0 ¼ S0trial Ycof ðS0 Þ Z1; (32)

vFmod 1 3S0 vU ¼ Dεp 1 þ Dεq þ DεU 3 vS vS 2Se

being Dεp, Dεq and DεU in the form:

3G 243 G J3 Dεq DεU ; Se 2S5e

Y¼

27G DεU ; S3e

Z¼

S2e Y ; 9 (41)

(33)

1 being the unit second-order tensor, and ðcofðS0 ÞÞij ¼ 12 ejkr eist ðS0 Þsk ðS0 Þtr the minors of ðS0 Þ, with eijk the Levi-Civita permutation symbols which allow the ﬂow rule dependent on U to be written as:

DEp ¼ Dl

(40)

with X, Y and Z given by:

X ¼1þ

with

vU 81 J3 3 S0 27 1 2 0 ¼ S $ þ cof ð S Þ þ 1 vS 2 S4e 2 Se 2S3e 9 e

(39)

where S0 can be written in the form:

p

vFmod vFmod vT 3S0 vFmod vU Þ þ þ þ vSe vT vSe 2Se vU vS

(38)

(34)

and cof ðS0 Þ, computing it from the expression given in Eq. (40), as:

X 2 YZ cof ðS0 Þ ¼ cof S0trial 2XZ þY 2 J3 S0 þ XYJ3 þ2Z 2 1

(42)

From Eq. (38), and after some algebra taking into account the identities:

cofðS0 Þ : cofðS0 Þ ¼

S4e ; 9

S2 cofðS0 Þ : 1 ¼ e 3

(43)

the following relations between the trial and current stress measures can be found-see Appendix A:

G. Vadillo et al. / European Journal of Mechanics A/Solids 56 (2016) 31e44

2 9GDεU 2 1 ðU þ 1Þ2 ¼ Se þ 3GDεq þ Se " 2S3e ðYSe Þ3 2ðU þ 1Þ2 1 ¼ ðU þ 1ÞX 3 þ 27 27

Strial e

J3trial

2

þX 2 ðYSe Þ þ with Strial ¼ e

X ¼1þ

ðU þ 1ÞX ðYSe Þ2 3

qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 3S0trial : S0trial ; 2

J¼

(44)

#

J3trial ¼ detðS0trial Þ, and

3G 9 GðU þ 1Þ Dεq DεU ; Se S2e

Y¼

27G DεU ; S3e

(45)

(49) ðnþ1Þ

For classical Gurson materials, an explicit expression of the tangent modulus consistent with the Euler backward algorithm has ndezbeen given by Aravas (1987), Zhang (1995), Vadillo and Ferna ez (2009). Following this procedure, the consistent stiffness Sa matrix for the modiﬁed GT model proposed in this work, J3 dependent, is obtained as follows (since all quantities in calculating J are referred to time (n þ 1), the superscript (n þ 1) will be dropped hereafter). For the convenience of the ﬁnite element implementation, J will be derived in matrix form. The boldface symbols will be used to denote matrices and vectors where:

vS ¼ fvS11 ; vS22 ; vS33 ; vS12 ; vS13 ; vS23 ; vS21 ; vS31 ; vS32 gT vE ¼ fvE11 ; vE22 ; vE33 ; vE12 ; vE13 ; vE23 ; vE21 ; vE31 ; vE32 gT

In a similar manner, it can be easily proved the relation:

Strial ¼ Sh þ KDεp h

vS vE

39

(50)

(46)

The set of ﬁve non-linear equations, involving only scalars, that should be solved to obtain the ﬁve unknown variables Dεp, Dεq, DεU, f and εp using an iterative NewtoneRaphson procedure, are:

vFmod vFmod vT vFmod vFmod vT Dεq ¼ 0; Dεp þ þ vSe vT vSe vSh vT vSh vF vFmod vFmod vT Dεq mod DεU ¼0 þ vU vSe vT vSe Sh Dεp þ Se Dεq ¼ ð1 f ÞsDεp Df ¼ ð1 f ÞDεp Fmod ðSe ; Sh ; T; U; s; f Þ ¼ 0 (47) with s ¼ sðεp Þ, and Sh, Se and U obtained from the relations:

Deriving Eq. (31) considering the relation given in Eq. (46): 0 vS ¼ vSh 1 þ vS0 ¼ vStrial h 1 KvDεp 1 þ vS

(51)

Deriving Eq. (40):

S0 vX þ XvS0 ¼ vS0trial vYcofðS0 Þ YvðcofS0 Þ vZ1;

(52)

1 and I0 being the vector and matrix mapping of the unit second order tensor and the unit deviatoric fourth-order tensor respectively. trial and vJ trial e see Eqs. vX, vY and vZ are functions of vStrial 3 h , vSe (B.4a), (B.7) and (B.9) from Appendix B. cof ðS0 Þ and vðcofS0 Þ are functions of S0trial and cofðS0trial Þ-see Eq. (42) and Eq. (B.71). Taking into account these relations, and clearing vS0 from Eq. (52) we have:

~ 1 þ Fv cofS0trial ~ S0trial þ E ~ cof S0trial þ E vS0 ¼ vS0trial þ E 1 2 3 (53)

Sh ¼ Strial KDεp h 2 2 9GDεU 2 1 ðU þ 1Þ2 ¼ Strial Se þ 3GDεq þ e Se " 2S3e ðYSe Þ3 2ðU þ 1Þ2 1 þ X 2 ðYSe Þ ðU þ 1ÞX 3 þ 27 27

~ ,E ~ and E ~ of the form: with E 1 2 3

~ vStrial þ E ~ vStrial þ E ~ vJ trial ~ ¼E E i i1 i2 i3 3 e h

(54)

(48)

#

ðU þ 1ÞX ðYSe Þ2 ¼ J3trial þ 3 and X and Y given by Eq. (45). Once the set of equations Eq. (47) are solved, Eqs. (40) and (42) allows ðS0 Þ to be written as function of 1 and the trial tensors S0trial and cof ðS0trial Þ. Finally, the updated stress S at time (n þ 1) can be calculated as S ¼ S h 1 þ S0 .

5.2. Consistent tangent modulus For inﬁnitesimal strain problems, Simo and Taylor (1985) showed that the use of a consistent tangent modulus J preserves the quadratic rate of asymptotic convergence of iterative solution schemes based on the Newton's method. This tangent operator deﬁnes the variation in stress at time (n þ 1) caused by a variation of the total strain as:

~ and F known. being all coefﬁcients E ij Introducing the relation (see Appendix B):

~ vStrial þ B ~ vStrial þ B ~ vJ trial vDεp ¼ B 11 12 13 3 e h

(55)

and the identities:

vStrial ¼ K ð1ÞT $vE h 3 0trial T vStrial ¼ S $vS0trial e 2Strial e T vJ3trial ¼ cof S0trial $vS0trial vS0trial ¼ 2GI0 $vE ¼ M$vS0trial v cof S0trial where M is a 9x9 matrix of the form:

(56)

40

G. Vadillo et al. / European Journal of Mechanics A/Solids 56 (2016) 31e44

2

0 6 trial 6 S33 6 trial 6 S 6 22 6 0 6 6 M¼6 0 6 6 Strial 32 6 6 0 6 6 4 0 Strial 23

Strial 33 0 Strial 11 0 Strial 31 0 0 Strial 13 0

Strial 22 Strial 11 0 Strial 21 0 0 Strial 12 0 0

0 0 Strial 21 0 0 Strial 31 Strial 33 Strial 23 0

0 Strial 31 0 0 0 0 Strial 32 Strial 22 Strial 21

Strial 32 0 0 Strial 31 0 0 0 Strial 12 Strial 11

0 0 Strial 12 Strial 33 Strial 32 0 0 0 Strial 13

into Eq. (51), the tangent modulus J can be written as:

T 0trial ~ þE ~ ~ $1T þ J ¼ K 1 KB 11 31 1$1 þ K E21 $cof S T 3G ~ 0trial ~ cof S0trial $ S0trial þ þE þ trial E 12 S 22 Se T ~ cof S0trial $I0 $cof S0trial ~ S0trial þ E þ 2G E 13 23

(58)

þ 2GðI0 þ F$M$I0 Þ To deﬁne this operator is not required any matrix inversion. The described algorithm as well as the corresponding tangent modulus has been implemented in the commercial ﬁnite element code ABAQUS/Standard (Simulia, 2014) through the user subroutine UMAT. 6. Comparison between the voided J2 cell and the modiﬁed continuum GT cell In order to analyse the accuracy of the proposed model, a selection of different loading and initial void volume fractions for Weldox 960 material will be studied in this section. The stressstrain and void volume fraction evolution within the deformation range 0 Ee Ec have been compared for the two RVE cell model approaches using three different triaxiality values (T ¼ 1, 1.5, 2) and two Lode parameters (L ¼ 0, 1) for the initial porosities f0 ¼ 0.005 and f0 ¼ 0.01. The case corresponding with L ¼ 1 should not be analysed in the sense that for this Lode value the modiﬁed GT model coincides with the classical GT model and the behaviour of GT and J2 voided cell are essentially the same as far as the qi parameters used for simulations were calibrated to minimize these differences. After a numerical iterative analysis, for the most critical stress and void volume fraction situations found in this work (f 0.08), convexity is assured if 0 kU 0.0403. Results for T ¼ 1 and L ¼ 0 are shown in Fig. 7 for f0 ¼ 0.005 (a)e(b) and f0 ¼ 0.01 (c)e(d) considering the J2 voided cell (dotted line) and the continuum GT Lode dependent model cell. Fig. 7(a) and (c) represent the evolution of the macroscopic effective stress Se normalized by the initial yield stress, s0, as a function of the macroscopic effective strain Ee, and Fig. 7(b) and (d) exhibit the porosity evolution f with Ee. The results of the simulations are plotted until reaching the coalescence deformation Ec. The ﬁtting parameters kU for the modiﬁed GT model simulations are kU ¼ 0.0, (which retrieves the classical GT model), 0.01, 0.03 and 0.04. The q1 and q2 parameters are the interpolated values obtained from Eq. (22) for T ¼ 1. Quantitative differences in the prediction of material ductile behaviour are observed for the modiﬁed GT model when different

0 Strial 13 0 Strial 23 Strial 22 Strial 12 0 0 0

3 Strial 23 7 0 7 7 0 7 7 0 7 7 7 7 Strial 21 7 7 Strial 11 7 trial 7 S13 7 7 0 5 0

(57)

kU values are used in the simulations. For kU ¼ 0.0 the modiﬁed GT model behaves underestimating the stress-strain curve of the voided J2 cell and overpredicting the void volume fraction evolution. The opposite tendency (overpredicting stress strain behaviour and underestimating porosity growth rate) is observed when kU is equal to 0.04. Then, with a proper choice of the kU parameter, it is possible to match the stress-strain and void growth rate curves of a GT-Lode dependent material to those predicted by the voided cell analysis. In this case kU ¼ 0.03 is the value that better ﬁts the behaviour of the material. Fig. 8 present analogous results for f0 ¼ 0.005 and f0 ¼ 0.01 prescribing in this case T ¼ 1 and L ¼ 1. The curves show that the proposed model, with a proper selection of kU (kU ¼ 0.03) agrees very well with that obtained from the voided cell analysis for both void volume fraction and stress-strain response. Similarly, in Figs. (9) and (10), where T ¼ 2, L ¼ 0 (Fig. 9(a)e(d)) and L ¼ 1 (Fig. 10(a)e(d)), the kU parameter that more accurately predict the stress-strain relations and void volume fraction evolution of the J2 voided cell is kU ¼ 0.03 for L ¼ 0 and a kU value within the range (0.01, 0.03) for L ¼ 1 for both initial porosities f0 ¼ 0.005 and f0 ¼ 0.01. The cases with triaxility T ¼ 1.5 and L ¼ 0 and L ¼ 1 lead to similar results. A ﬁnal remark is that the proposed new approach and the calibrated (q1mod, q2mod) values improve the Gurson model but it is still imperfect. It is obvious that further numerical studies and comparisons with experimental results are necessary to further verify/calibrate the proposed modiﬁcation of the Gurson model.

7. Concluding remarks The salient feature of the present paper is the proposition of an improved GT model that accounts for the triaxiality and Lode effects through q1 and q2. We also present the ﬁnite element implementation of the modiﬁed GT model using return mapping method (Euler-backward integration technique) and the formulation of the consistent tangent modulus. An extension of the computational cell model employed by Xia and Shih (1995a,b, 1996) has been developed to prescribe both macroscopic triaxiality and Lode parameter, and several numerical simulations are presented for Weldox 960 steel with different initial porosities and for distinct prescribed T and L values. The q1 and q2 classical GT parameters have been calibrated for L ¼ 1 and extended to other possible Lode parameters values. The convexity of the proposed yield modiﬁed Gurson locus is assured. The obtained results show good agreement between the two cell models (the voided J2 and the proposed continuum damage model cells) for the triaxialities and Lode parameters tested (T ¼ 1, 1.5, 2 and L ¼ 0, 1).

G. Vadillo et al. / European Journal of Mechanics A/Solids 56 (2016) 31e44

Fig. 7. Se versus Ee and f versus Ee for f0 ¼ 0.005 (a, b) and f0 ¼ 0.01 (c, d). T ¼ 1, L ¼ 0.

Fig. 8. Se versus Ee and f versus Ee for f0 ¼ 0.005 (a, b) and f0 ¼ 0.01 (c, d). T ¼ 1, L ¼ 1.

41

42

G. Vadillo et al. / European Journal of Mechanics A/Solids 56 (2016) 31e44

Fig. 9. Se versus Ee and f versus Ee for f0 ¼ 0.005 (a, b) and f0 ¼ 0.01 (c, d). T ¼ 2, L ¼ 0.

Fig. 10. Se versus Ee and f versus Ee for f0 ¼ 0.005 (a, b) and f0 ¼ 0.01 (c, d). T ¼ 2, L ¼ 1.

G. Vadillo et al. / European Journal of Mechanics A/Solids 56 (2016) 31e44

At high triaxialities, the proposed modiﬁed GT model permits to extend predictions to any Lode parameter and expands its applicability in order to have better agreement with the J2 ﬁnite element analyses with a unitary voided cell.

43

vDεp ¼ B11 vStrial þ B12 vStrial þ B13 vU e h þ B22 vStrial þ B23 vU vDεq ¼ B21 vStrial e h vDεU ¼ B31 vStrial þ B32 vStrial þ B33 vU; e h

Bij coefficients known (B.2)

Acknowledgements The authors are indebted to the Ministerio de Economía y Competitividad (Projects DPI2011-23191 and DPI/2011-24068) for the ﬁnancial support received which allowed condicting part of this work. The authors would like to thank Professor J. Faleskog, Royal Institute of Technology (KTH) of Sweden, and Dr. J.A. RodríguezMartínez and Dr. J. Zahr, University Carlos III of Madrid (UC3M), for valuable discussions.

From the derivation of Eq. (48.c):

ðYS Þ2 e vðYSe Þ 3ðU þ 1ÞX 2 vX þ X 3 vU þ 2ðU þ 1Þ2 1 9 þ4

ðYSe Þ3 ðU þ 1ÞvU þ þ2X ðYSe Þ þ X 2 vðYSe Þ 27

ðYSe Þ2 2X ðU þ 1Þ X ðYSe Þ2 ðU þ 1ÞvX þ vU ðYSe ÞvðYSe Þ þ 3 3 3 27 trial 81J3trial ¼ vJ3 vSe 2S4e 2S3e þ

Appendix A 0

0

Operating S trial : S trial from Eq. (38) considering the identities given in Eq. (37) and Eq. (43), it follows:

(B.3) being vX and v(YSe) the derivades of X and (YSe) from Eq. (45):

Strial e

2

2 ¼ Se þ 3GDεq þ ð2GDεU Þ2

27

2S2e

! 3$812 J32 3 $ 8 S8e 2

vDεq 9GðU þ 1Þ 9GDεU vDεU vU Se S2e S2e ! Dεq 18GðU þ 1ÞDεU 3G 2 vSe þ S3e Se

vX ¼ 3G

(A.1)

Taking into account the relation S0 : cofðS0 Þ ¼ 3J3 , Eqs. (40) and (42) allows J3trial to be written as function of the stress measures J3 and Se as:

J3trial

(A.2)

27

vSe þ

27G S2e

vDεU

vU can be written after operating in Eqs. (B.3), (B.1b) and (B.4) as:

(B.5)

or in a similar manner, considering the relation given in Eqs. (B.2b, B.2c):

~ vStrial þ B ~ vStrial þ B ~ vJ trial vU ¼ B 41 42 43 3 e h

3G 243 G J3 27G S2 Y X ¼1þ Dεq DεU ; Y ¼ 3 DεU ; Z ¼ e ; J3 Se 9 2S5e Se ¼

S3e

3

being X, Y, Z and J3:

2S3e

54GDεU

vU ¼ B41 vDεq þ B42 vDεU þ B43 vStrial þ B44 vJ3trial e

2 6 2 J S2 X Y 2 Se þ X 2 Y S4e þ 3 e ¼ J3 X þ Y J32 729 27 3 3

vðYSe Þ ¼

(B.4)

(B.6)

that allows vDεp, vDεq and vDεU to be written as:

~ vStrial þ B ~ vStrial þ B ~ vJ trial vDεp ¼ B 11 12 13 3 e h ~ vStrial þ B ~ vStrial þ B ~ vJ trial vDεq ¼ B 21 22 23 3 e h ~ vStrial þ B ~ vStrial þ B ~ vJ trial vDεU ¼ B 31 32 33 3 e h

ðU þ 1Þ

~ values known B ij (B.7)

Deriving the relation given in Eq. (42):

Appendix B Deriving Eq. (48aeb), vSh and vSe have the form.

vSh ¼ vStrial KvDεp ; h vSe ¼ A11 vStrial þ A12 vDεq þ A13 vDεU e þA14 vU; Aij coefficients known

(B.1)

and the values vDεp, vDεq and vDεU obtained from the ﬁve implicit constitutive equations given in Eq. (47) and the relations obtained in Eq. (B.1):

ð2XvX YvZ ZvY Þcof ðS0 Þ þ X 2 YZ vðcofS0 Þ ¼ v cofS0trial 2ZvX þ 2XvZ þ 2YJ3 vY þ Y 2 vJ3 S0 2XZ þ Y 2 J3 vS0 þ ðYJ3 vX þ XJ3 vY þ XYvJ3 þ 4ZvZ Þ1 (B.8) with vX given in Eq. (B.4a), and vY and vZ obtained from Eq. (A.3) and with the form:

44

vY ¼

G. Vadillo et al. / European Journal of Mechanics A/Solids 56 (2016) 31e44

27G S3e

vDεU

81G S4e

vSe ;

S2 2YSe vSe vZ ¼ e vY þ 9 9

(B.9)

and vJ3 as:

vJ3 ¼

6S2e ðU þ 1Þ 2S3e vSe þ vU 27 27

(B.10)

it is possible to obtain, considering Eqs. (B.1a), (B.4a) (B.6), (B.7), (B.8), (B.9) and (B.10):

~ vS0 þ D ~ v cofS0trial þ C ~ S0 þ De cof ðS0 Þ þ D ~ 1 vðcofS0 Þ ¼ C 1 2 1 2 3 (B.11) ~ , D ~ and D ~ of the form: D ~ ¼D ~ vStrial þ D ~ vStrial being D 1 2 3 i i1 i2 e h ~ ,C ~ and all D ~ vJ trial with C ~ coefﬁcients known. þD 1 2 i3 3 ij References Aravas, N., 1987. On the numerical integration of a class of pressure-dependent plasticity models. Int. J. Numer. Methods Eng. 24, 1395e1416. Bai, Y., Wierzbicki, T., 2008. A new model of metal plasticity and fracture with pressure and Lode dependence. Int. J. Plast. 24, 1071e1096. Bao, Y., Wierzbicki, T., 2004. On fracture locus in the equivalent strain and stress triaxiality space. Int. J. Mech. Sci. 46, 81e98. Barsoum, I., Faleskog, J., 2007. Rupture mechanisms in combined tension and shear: micromechanics. Int. J. Solids Struct. 44, 5481e5498. Barsoum, I., Faleskog, J., 2011. Micromechanical analysis on the inﬂuence of the Lode parameter on void growth and coalescence. Int. J. Solids Struct. 48, 925e938. Barsoum, I., Faleskog, J., Pingle, S., 2011. The inﬂuence of the Lode parameter on ductile failure strain in steel. Procedia Eng. 10, 69e75. Benallal, A., Desmorat, R., Fournage, M., 2014. An assessment of the role of the third stress invariant in the gurson approach for ductile fracture. Eur. J. Mech. A/ Solids 47, 400e414. Benzerga, A., 2002. Micromechanics of coalescence in ductile fracture. J. Mech. Phys. Solids 50, 1331e1362. Besson, J., 2010. Continuum models of ductile fracture: a review. Int. J. Damage Mech. 19, 3e52. Brünig, M., Chyra, O., Albrecht, D., Driemeier, L., Alves, M., 2008. A ductile damage criterion at various stress triaxialities. Int. J. Plast. 24, 1731e1755. ~ eda, P., 2012. Inﬂuence of the Lode parameter and the stress Danas, K., Ponte-Castan triaxiality on the failure of elasto-plastic porous materials. Int. J. Solids Struct. 49, 1325e1342. Faleskog, J., Gao, X., Shih, C., 1998. Cell model for nonlinear fracture analysis I. micromechanics calibration. Int. J. Fract. 89 (4), 355e373. Flandi, L., Leblond, J.B., 2005. A new model for porous viscoplastic solids incorporating void shape effects II: numerical validation. Eur. J. Mech. 24, 552e571. Gao, X., Faleskog, J., Shih, C.F., 1998. Ductile tearing in part-throgh cracks: experiments and cell-model predictions. Eng. Fract. Mech. 59, 761e777. Gao, X., Kim, J., 2006. Modeling of ductile fracture: signiﬁcance of void coalescence. Int. J. Solids Struct. 43, 6277e6293. Gao, X., Whang, T., Kim, J., 2005. On ductile fracture initiation toughness: effects of void volume fraction, void shape and void distribution. Int. J. Solids Struct. 42, 5097e5117. Gao, X., Zhang, T., Hayden, M., Roe, C., 2009. Effects of the stress state on plasticity and ductile failure of an aluminum 5083 alloy. Int. J. Plast. 25, 2366e2382. Gao, X., Zhang, T., Zhou, J., Graham, S.M., Hayden, M., Roe, C., 2011. On stress-state dependent plasticity modeling: signiﬁcance of the hydrostatic stress, the third invariant of stress deviator and the non-associated ﬂow rule. Int. J. Plast. 27, 217e231. Gologanu, M., Leblond, J., Perrin, G., Devaux, J., 1997. Recent extensions of Gursons model for porous ductile metals. In: Suquet, P. (Ed.), Continuum Micromechanics. Springer Verlag.

ra jeu, M., Michel, J.-C., Suquet, P., 2000. A micromechanical approach of damage Ga in viscoplastic materials by evolution in size shape and distribution of voids. Comput. Methods Appl. Mech. Eng. 183, 223e246. Gurson, A.L., 1977. Continuum theory of ductile rupture by void nucleation and growth part I. yield criteria and ﬂow rules for porous ductile media. J. Eng. Mater. Technol. 99, 2e15. Hill, R., 1967. The essential structure of constitutive laws for metal composites and polycrystals. J. Mech. Phys. Solids 15, 79e95. Jackiewicz, J., 2011. Use of a modiﬁed Gurson model approach for the simulation of ductile fracture by growth and coalescence of microvoids under low, medium and high stress triaxiality loadings. Eng. Fract. Mech. 78, 487e502. Kim, J., Gao, X., Srivatsan, T.S., 2003. Modeling of crack growth in ductile solids: a three-dimensional analysis. Int. J. Solids Struct. 40, 7357e7374. Kim, J., Gao, X., Srivatsan, T.S., 2004. Modeling of void growth in ductile solids: effects of stress triaxiality and initial porosity. Eng. Fract. Mech. 71, 379e400. Kim, J., Zhang, G., Gao, X., 2007. Modeling of ductile fracture: application of the mechanism-based concepts. Int. J. Solids Struct. 44, 1844e1862. Koplik, J., Needleman, A., 1988. Void growth and coalescence in porous plastic solids. Int. J. Solids Struct. 24, 835e853. McClintock, F.A., 1968. A criterion for ductile fracture by the growth of holes. J. Appl. Mech. 35, 363e371. Monchiet, V., Cazacu, O., Charkaluk, E., Kondo, D., 2008. Macroscopic yield criteria for plastic anisotropic materials containing spheroidal voids. Int. J. Plast. 24, 1158e1189. Nahshon, K., Hutchinson, J.W., 2008. Modiﬁcation of the Gurson model for shear failure. Eur. J. Mech. A/Solids 27, 1e17. Pardoen, T., Hutchinson, J.W., 2000. An extended model for void growth and coalescence. Int. J. Mech. Phys. Solids 48, 2467e2512. Pietryga, M., Vladimirov, I., Reese, S., 2012. A ﬁnite deformation model for evolving ﬂow anisotropy with distortional hardening including experimental validation. Mech. Mater. 44, 163e173. Pineau, A., Pardoen, T., 2007. Comprehensive Structural Integrity Encyclopedia, vol. 2. Elsevier, Amsterdam (chapter 6). Rice, J.R., Tracey, D.M., 1969. On the ductile enlargement of voids in triaxial stress ﬁelds. J. Mech. Phys. Solids 17, 201e217. Simo, J., Taylor, R.L., 1985. Consistent tangent operators for rate-independent elastoplasticity. Comput. Methods Appl. Mech. Eng. 48, 101e118. Simulia, 2014. ABAQUS/Standard User's Manual, Version 6.14 Edition. Dassault mes, Providence, USA. Syste Tvergaard, V., 1981. Inﬂuence of voids on shear band instabilities under plane strain conditions. Int. J. Fract. 17, 389e407. Tvergaard, V., 1982. On localization in ductile materials containing spherical voids. Int. J. Fract. 18, 237e252. ez, J., 2009. An analysis of Gurson model with parameters Vadillo, G., Fern andez-Sa dependent on triaxiality based on unitary cells. Eur. J. Mech. A/Solids 28, 417e427. Wen, J., Huang, Y., Hwang, K.C., Liu, C., Li, M., 2005. The modiﬁed Gurson model accounting for the void size effect. Int. J. Plast. 21, 381e395. Xia, L., Shih, C.F., 1995a. Ductile crack growth e I. A numerical study using computational cells with microstructurally based length scales. J. Mech. Phys. Solids 43, 233e259. Xia, L., Shih, C.F., 1995b. Ductile crack growth e II. Void nucleation and geometry effects on macroscopicvfracture behavior. J. Mech. Phys. Solids 43, 1953e1981. Xia, L., Shih, C.F., 1996. Ductile crack growth e III. Transition to cleavage fracture incorporating statistics. J. Mech. Phys. Solids 44, 603e639. Xue, L., 2007. Damage accumulation and fracture initiation in uncracked ductile solids subject to triaxial loading. Int. J. Solids Struct. 44, 5163e5181. Xue, L., 2008. Constitutive modeling of void shearing effect in ductile fracture of porous materials. Eng. Fract. Mech. 75, 3343e3366. Yamamoto, H., 1978. Conditions for shear localization in the ductile fracture of void containing materials. Int. J. Fract. 14, 347e365. Zhang, K.S., Bai, J.B., François, D., 2001. Numerical analysis of the inﬂuence of the Lode parameter on void growth. Int. J. Solids Struct. 38, 5847e5856. Zhang, Z.L., 1995. On the accuracies of numerical integration algorithms for Gursonbased pressure-dependent elastoplastic constitutive models. Comput. Methods Appl. Mech. Eng. 121, 15e28. Zhang, Z.L., Thaulow, C., Ødegård, J., 2000. A complete Gurson model approach for ductile fracture. Eng. Fract. Mech. 67, 155e168.

Copyright © 2023 COEK.INFO. All rights reserved.